Biogenic synthesis of magnesium oxide nanoparticles using Manihot esculenta (Crantz) leaf extract
- 102 Downloads
Recently, plant-mediated route or green approach for preparing metal and metal oxide nanoparticles has received enormous attention due to the ease of preparation and environmental friendliness when compared to physical and chemical methods. Plants contain phytochemicals which have been proposed as bio-reductants and capping agents for forming metal nanoparticles. Therefore, this study was aimed to prepare magnesium oxide nanoparticles (MgONPs) using aqueous extract of Manihot esculenta leaf. The leaf extract was first analyzed in a gas chromatograph–mass spectrometer (GC–MS) to examine the phytochemicals present. Then, the MgONPs formed were evaluated using UV–Visible (UV–Vis) spectrophotometry, scanning electron microscopy (SEM), energy-dispersive X-ray analysis (EDX), transmission electron microscopy (TEM), X-ray diffractometry (XRD) and Fourier transform infrared (FTIR) spectroscopy, to confirm the formation of MgONPs and to determine the morphology, elemental composition, shape and size, phase composition and nature of bonds present in the sample. Results revealed the formation of monodisperse, hexagonal shaped MgONPs of average size 36.7 nm having potentials for application in catalysis and as antimicrobial agent. Hence the process reported herein could be optimized for large-scale preparation of MgONPs.
KeywordsMonodisperse Manihot esculenta Green synthesis Magnesium oxide nanoparticles Capping agent
Nanotechnology is a promising field of Materials Science that is capable of producing materials of various types at the nanoscale level. Nanoparticles are a wide class of materials that include particulate substances having dimension 1–100 nm . In recent times, metal nanoparticles research has attracted immense attention due to their unusual properties compared to bulk metals , because at the nanoscale, various physiochemical properties can be severely influenced. Metal nanoparticles have wide biomedical and pharmaceutical applications as alternative antimicrobial agents due to the reemergence of infectious diseases and the appearance of antibiotic-resistant strains. Magnesium nanoparticles (MgONPs), in particular, have been applied in catalysis, toxic waste remediation, paints, superconducting products, optical, electrical, electronics, antiseptics, antibacterial activities, semiconductors and catalytic devices .
Generally, conventional chemical synthesis methods of nanoparticles, besides being expensive, pose various health and environmental risks  due to the toxic nature of some of the starting reagents and by-products associated with these methods.
Synthesis of metal nanoparticles using plant extracts is attracting increasing interest as an alternative approach. Biologically synthesized metal nanoparticles via plant-mediated pathway have the benefits of being facile, nontoxic and ecofriendly. Biomolecules present in plant extracts act as reducing and capping agents, forming stable nanoparticles. Thus, the properties of the obtained metal nanoparticles, such as biocompatibility and antimicrobial activity, also depend on the properties of the various phytochemicals present in the plant extracts from which they were synthesized.
There are a number of reports on the preparation of MgONPs via plant-mediated route. Jhansi et al.  prepared MgONPs in various nanometer sizes using white button mushroom aqueous extract and studied their effects on peanut (Arachis hypogaea L.) seed germination. Of the different three sample sizes studied, the one with the least particle size gave the greatest enhancement in seed germination. This, they suggested was due the more efficient penetration of the MgONPs into the seed coat to promote Mg content and water uptake needed for germination. Abdallah et al.  synthesized MgO nano-flowers using aqueous extracts from Rosmarinus officinalis L. (Rosemary) flowers as the reducing agent. The obtained MgO nano-flowers showed significant antimicrobial effect against Xanthomonas oryzae pv. oryzae, Furthermore, in the report of Vergheese and Vishal , MgONPs were synthesized from aqueous leaf extract of Trigonella foenum-graceum and tested for its antimicrobial activity against the Gram-positive E. Coli, Gram-negative S. aereus and Bacillus bacteria. The MgONPs showed potency against E. Coli and S. aereus at a similar concentration, but in the case of Bacillus double dosage was required to achieve a similar effect.
Manihot esculenta is extensively cultivated as an annual crop in the tropical and subtropical regions of the world for its edible starchy tuberous root, a major source of food carbohydrates in the tropics. Cassava, the tubers from the plant, is a major staple food in the developing world, providing a basic diet for over half a billion people . The leaf contains vitamins A, B1, calcium, calories, phosphorus, protein, fat, carbohydrate and iron. It can be used to treat measles, small pox, chicken pox, skin rashes, fevers and headaches, colds, constipation, ringworm, tumor, conjunctivitis, sores and abscesses . Furthermore, chlorophyll in the leaves serves as antioxidant and anticancer agent. These health attributes of Manihot esculenta leaf may be attributed to the phytochemicals present.
Even though the tubers of Manihot esculenta serve as staple food for the teaming population in some developing countries where the crop is cultivated on a large scale, the leaf is not well known to serve as a major source of vegetable. Thus, it is often discarded as waste after harvesting the tubers. It is against this backdrop, therefore, and given the large-scale cultivation of this crop in many parts of the world, that the present work is designed to prepare MgONPs using Manihot esculenta leaf extract as the reducing agent towards a potential commercial scale, ecofriendly synthesis of MgONPs. To best of our knowledge there is no current report on the synthesis of MgONPs from Manihot esculenta leaf.
Materials and methods
The Manihot esculenta leaves used for this study were collected from the premises of Bells University of Technology, Ota, Ogun State, South-west, Nigeria. Mg(NO3)2·6H2O and absolute ethanol were purchased from Sigma-Aldrich.
Preparation of Manihot esculenta aqueous leaf extract
The leaves of Manihot esculenta were washed with tap water and then rinsed with deionized water to get rid of dust and particulate impurities. Afterwards, they were sun-dried and pulverized into fine powder to confer a large surface for absorption. Then, 48 g of the powder was mixed with 250 mL of deionized water in a 500 mL capacity conical flask. The mixture was sealed and boiled for 15 min in a thermostatic water bath. After allowing to cool to room temperature, it was filtered to obtain the aqueous extract. The extract was stored in a refrigerator between 5 and 10 °C for further use.
Synthesis of MgONPs
250 mL of the Manihot esculenta aqueous leaf extract was added in drops to 50 mL of 0.1 M solution of Mg(NO3)2·6H2O in a 500 mL capacity beaker under a constant stirring condition with a magnetic stirrer. The total time consumed for the addition was 12 h. The obtained solid–liquid dispersion was then centrifuged at 7000 rpm for 10 min. After this, the supernatant was discarded and the residue washed with deionized water to remove excess Mg(NO3)·6H2O and residual organic molecules. Furthermore, it was dried in an oven at 70 °C for 2 h and then calcined in a furnace at 500 °C for 3 h to obtain MgONPs. Finally, the obtained MgONPs were sonicated at 40 °C for 1 h in an ultrasonic cleaner (CLEAN-120HD) to disperse the particles.
To identify the phytochemicals responsible for the reduction reaction and stabilization of the formed MgONPs, the Manihot esculenta aqueous leaf extract was analyzed in a gas chromatograph–mass spectrometer (GC–MS) (Shimadzu QP2010SE) at a 1:1 injection ratio of the ethanolic solution of the extract into the machine. Thereafter, the phytochemicals were identified based on their fragmentation patterns via a database incorporated into the GC–MS machine. MgONPs formation in the reaction mixture between Mg(NO3)2·6H2O and the Manihot esculenta aqueous leaf extract was confirmed using UV–Vis absorption spectrophotometer (Uniscope SM 7504) in the wavelength between 100 and 700 nm.
Morphological study to assess the microstructure, particle distribution and elemental composition of the MgONPs was performed in a scanning electron microscope (SEM) equipped with an energy-dispersive X-ray analyzer (EDX) unit (SEM: JEOL JSM 7660F). The sample was analyzed with an accelerating voltage of 15 kV.
The particle size and structure of the MgONPs were determined by transmission electron microscopy (TEM) (TEM: JEM-ARM200F-G) using 200 kV accelerating voltage. Then, the average particle size was determined from the SEM and TEM micrographs using ImageJ software.
The diffraction pattern of the MgONPs was evaluated in an X-ray diffractometer (XRD) (XRD: Rigaku D/Max-IIIC) to study the type of phases present in the sample and to assess the crystalline structure of the MgONPs.
Fourier transform infrared (FTIR) spectroscopy (FTIR: Nicolet iS10) with wavenumber in the range 350–4000 cm−1 was employed to assess the type of bonds present in the MgONPs so as to complement and confirm the result of the analysis with GC–MS, UV and XRD.
Results and discussion
Microstructural characteristics and elemental composition of the MgONPs
The particles size of the MgONPs obtained in this study falls between 35.9–47.3 nm, but closer to 35.9 nm, hence should exhibit a comparable effect against Bacillus subtilis var. niger. Besides, the surface morphology exhibited by the MgONPs could be beneficial for catalysis application  as well as offer optical and other medicinal values . The large surface area implies that in heterogeneous catalysis, the MgONPs should function as the metal , therefore, resulting in improved performance compared with the bulk material.
Particle shape and size
The properties exhibited by the MgONPs may be the result of the efficient capping ability of the phytochemicals present in the plant extract together with the ultrasonic radiation passed through the sample in ethanol medium, which improved dispersion and homogeneity of the particles . Efficient dispersion of particles affects their interaction with test media in various in vitro and in vivo experiments, such as cytotoxicity  and in supported heterogeneous catalysis [16, 17, 18].
Diffraction pattern of the MgONPs
Bond properties of the MgONPs
The prominent peak at 1382 cm−1 is assigned to Mg–O vibration  while the small peaks located at 1041 and 941 are associated with C–O and C–O–C diagnostic bonds, respectively . The peak observed around 829 cm−1 indicates the formation of hexagonal MgONPs [21, 23, 24], in agreement with the SEM, TEM and XRD results.
Monodisperse MgO nanoparticles have been successfully synthesized based on the green approach using Manihot esculenta aqueous leaf extract. GC–MS identified several organic biomolecules proposed to act as reductant and capping agents to form the MgO nanoparticles. Analysis conducted using UV–Vis spectrophotometry, SEM/EDX, TEM, XRD and FTIR confirmed the formation of hexagonal shaped MgONPs of average diameter of 36.7 nm. One of the significances of this study is the use of the Manihot esculenta plant-mediated route which makes the process economical and more ecologically friendly, compared to chemical synthesis. In addition, Manihot esculenta, because it is grown in many developing countries in large quantities, where the tubers serve as a source of cassava, a staple food, implies that the leaves would be widely available for a potential commercial scale preparation of MgONPs, since they do not serve as dependable source of vegetable. Finally, based on the protocol established in this study, it is possible to obtain monodisperse MgO nanoparticles with shape and size uniformity.
The authors are grateful to the Department of Food and Chemical Sciences, Bells University of Technology, Ota for providing technical support for this work.
Compliance with ethical standards
Conflict of interest
The authors report no conflict of interest.
- 3.Rao, K.G., Ashok, C.H., Venkateshwara, R.K., Chakra, C.H.S.: Structural properties of MgO NPs, synthesized by Co-precipitation technique. Int. J. Sci. Res. 3(12), 43–46 (2014)Google Scholar
- 6.Abdallah, Y., Ogunyemi, S.O., Abdelazez, A., Zhang, M., Hong, X., Ibrahim-Hossain, A., Fouad, H., Li, B., Chen, J.: The green synthesis of MgO nano-Flowers using Rosmarinus officinalis L. (Rosemary) and the antibacterial activities against Xanthomonas oryzae pv. oryzae. BioMed Res. Int. 209, 5620989 (2019)Google Scholar
- 7.Vergheese, M., Kiran-Vishal, S.: Green synthesis of magnesium oxide nanoparticles using Trigonella foenum-graecum leaf extract and its antibacterial activity. J. Pharmacogn. Phytochem. 7, 1193–1200 (2018)Google Scholar
- 8.Thambi, M., Cherian, T.: Pesticidal activity of the leaves of Manihot esculenta against the pest Sitophilus oryzae. Pharma Innov. J. 4, 15–18 (2015)Google Scholar
- 9.Rahalison, L., Gupta, M.P., Santana, A.I.: Screening for antifungal activity of Panamanian plants. J. Pharmacol. 31, 68–76 (1993)Google Scholar
- 11.Huang, J., Chen, C., He, N., Hong, J., Lu, Y., Qingbiao, L., Shao, W., Sun, D., Wang, X.H., Wang, Y., Yiang, X.: Biosynthesis of silver and gold nanoparticles by novel sundried Cinnamomum camphora leaf. Nanotechnology 18, 105–106 (2007)Google Scholar
- 12.Lei, H., Dianqing, L., Yanjun, L., Evans, D.G., Xue, D.: Influence of nano-MgO particle size on bactericidal action against Bacillus subtilis var, niger. Chin Sci. Bull. 50, 514–519 (2005)Google Scholar
- 14.Astruc, D.: Nanoparticles and catalysis. Wiley, New York (2008)Google Scholar
- 15.Kaur, I., Ellis, L.-J., Romer, I., Tantra, R., Carriere, M., Allard, S., Mayne-L’Hermite, M., Minelli, C., Unger, W., Potthoff, A., Rades, S., Valsami-Jones, E.: Dispersion of nanomaterials in aqueous media: towards protocol optimization. J. Vis. Exp. 130, 56074 (2017)Google Scholar
- 17.Boudart, M.: Catalysis by supported metals. In: Frankenburg, W.G. (ed.) Advances in catalysis, pp. 153–166. Academic Press, New York (1969)Google Scholar
- 21.Viswanatha, R., Venkatesh, T.G., Vidyasagar, C.C., Nayaka, A.: Preparation and Characterization of ZnO and Mg–ZnO nanoparticle. Arch. Appl. Sci. Res. 4, 480–486 (2012)Google Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.